Surface Treatments Coatings, and Cleaning
The preceding chapters have described methods of producing desired shapes from a Wide variety of materials; although material and process selection is very important, often the surface properties of a component determine its performance or commercial success. This chapter describes various surfacefinishing operations that can be performed for technical and aesthetic reasons subsequent to manufacturing a part. The chapter presents the surface treatment, cleaning, and coating processes that are commonly performed and includes a discussion of mechanical surface treatments such as shot peening, laser peening, and roller burnishing, with the benefit of imparting compressive residual stresses onto metal surfaces. Coating operations are then examined, including cladding, thermal spray operations, physical and chemical vapor deposition, ion implantation, and electroplating. The benefits of diamond and diamond-like carbon coatings are also investigated.
Finally, surface-texturing, painting, and cleaning operations are described.
34.I 34.2 34.3 34.4
34.7 34.8 34.9
34.l0 34.I! 34.l2 34.I3
After a part is manufactured, some of its surfaces may have to be processed further in order to ensure that they receive certain properties and characteristics, It may be necessary to perform surface treatments in order to °
Improve resistance to wear erosion, and indentation (e.g., for machine-tool slidevvays, as shown in Figs. 23.2 and 35.1, Wear surfaces of machinery, and shafts, rolls, cams, and gears) Control friction (on sliding surfaces of tools, dies, bearings, and machine Ways)
° ° °
Introduction 973 Mechanical Surface Treatments 974 Mechanical Plating and Cladding 976 Case Hardeningand
34.I4 34.I5 34.I6
Thermal Spraying 977 Vapor Deposition 979 Ion lmplantation and Diffusion Coating 982 LaserTreatments 982 Electroplating, Electroless Plating, and Electroforming 983 Conversion Coatings 986 Hot Dipping 987 Porcelain Enameling; Ceramic and Organic Coatings 988 Diamond Coating and Diamond-like Carbon 989 Surface Texturing 990 Painting 990 Cleaning of Surfaces 99|
Repair ofaWorn Turbine-engine Shaft by Thermal Spraying 979 Applications of Laser Surface Engineering 983 Ceramic Coatings for High-temperature Applications 989
Reduce adhesion (of electrical contacts) Improve lubrication (surface modification to retain lubricants) Improve resistance to corrosion and oxidation (on sheet metals for automobile bodies, gas-turbine components, food packaging, and medical devices)
Surface Treatments, Coatings, and Cleaning
° ° ° °
Improve fatigue resistance (of bearings and shafts with fillets) Rebuild surfaces (on worn tools, dies, molds, and machine components) Modify surface texture (appearance, dimensional accuracy, and frictional characteristics) Irnpart decorative features (color and texture).
Numerous techniques are used to impart these characteristics to various types of metallic, nonmetallic, and ceramic materials on the basis of mechanisms that involve (a) plastic deformation of the workpiece surface, (b) chemical reactions, (c) thermal means, (d) deposition, (e) implantation, and (f) organic coatings and paints. We begin with surface-hardening techniques and then continue with descriptions of different types of coatings that are applied to surfaces by various means. Some of these techniques also are used in the manufacture of semiconductor devices, as described in Chapter 28. Techniques that are used to impart texture on workpiece surfaces and types of organic coatings used for various purposes are then described. The chapter ends with a discussion of methods used for cleaning manufactured surfaces before the components are assembled into the completed product and made ready for service. Environmental considerations regarding the fluids used and the waste material from various surface-treatment processes are also included, as they are an important factor to be considered.
Mechanical Surface Treatments
Several techniques are used to mechanically improve the surface properties of manufactured components. The more common methods are the following:
Shot Peening. In shot peening, the workpiece surface is impacted repeatedly with a large number of cast steel, glass, or ceramic shot (small balls), which make overlapping indentations on the surface. This action, using shot sizes that range from 0.125 to 5 mm in diameter, causes plastic surface deformation at depths up to 1.25 mm. Because the plastic deformation is not uniform throughout the part’s thickness, shot peening causes compressive residual stresses on the surface, thus improving the fatigue life of the component by delaying the initiation of fatigue cracks. Unless the process parameters are controlled properly, the plastic deformation of the surface can be so severe that it can damage the surface. The extent of deformation can be reduced by gravity peening, which involves larger shot sizes, but fewer impacts on the workpiece surface. Shot peening is used extensively on shafts, gears, springs, oil-well drilling equipment, and jet-engine parts, such as turbine and compressor blades. However, note that if these parts are subjected to high temperatures, the residual stress will begin to relax (thermal relaxation) and their beneficial effects will be diminished greatly. An example is gas-turbine blades performing at their operating temperatures. Laser Shot Peening. In this process, also called laser shock peening and first developed in the mid-19605 (but not commercialized until much later), the workpiece surface is subjected to planar laser shocks (pulses) from high-power lasers. This surface-treatment process produces compressive residual-stress layers that are typically 1 mm deep with less than 1% of cold working of the surface. Laser peening has been applied successfully and reliably to jet-engine fan blades and to materials such as titanium, nickel alloys, and steels for improved fatigue resistance and some corro-
Mechanical Surface Treatments
sion resistance. Laser intensities necessary for the process are on the order of 100 to 300 ]/cmz and have a pulse duration of about 30 nanoseconds. Currently, the basic limitation of laser shot peening for industrial, cost-effective applications is the high cost of the high-power lasers (up to 1 kW) that must operate at energy levels of 100 J/pulse.
Water-jet Peening. In this more recently developed process,
a Water jet at pressures as high as 400 MPa impinges on the surface of the workpiece, inducing compressive residual stresses and surface and subsurface hardening at the same level as in shot peening. The water-jet peening process has been used successfully on steels and aluminum alloys. The control of process variables (jet pressure, jet velocity, the design of the nozzle, and its distance from the surface) is important in order to avoid excessive surface roughness and surface damage.
This process uses a hand tool based on a piezoelectric transducer. Operating at a frequency of 22 kHz, it can have a variety of heads for different applications.
Roller Burnishing. In this process, also called surface rolling, the surface of the component is cold worked by a hard and highly polished roller or set of rollers. The process is used on various flat, cylindrical, or conical surfaces (Fig. 34.1). Roller burnishing improves surface finish by removing scratches, tool marks, and pits and induces beneficial compressive surface residual stresses. Consequently, corrosion resistance is improved, since corrosive products and residues cannot be entrapped. In a variation of this process called low-plasticity burnishing, the roller travels only once over the surface, inducing residual stresses and minimal plastic deformation. Internal cylindrical surfaces also are burnished by a similar process, called ballizing or ball burnishing. In this process, a smooth ball (slightly larger than the bore diameter) is pushed through the length of the hole. Roller burnishing is used to improve the mechanical properties of surfaces as Well as their surface finish. It can be used either by itself or in combination with other finishing processes, such as grinding, honing, and lapping. The equipment can be mounted on various CNC machine tools for improved productivity and consistency of performance. All types of metals (soft or hard) can be roller burnished. Roller burnishing is typically used on hydraulic-system components, seals, valves, spindles, and fillets on shafts.
Burnishing tools and roller burnishing of (a) the fillet of induce compressive surface residual stresses for improved fatigue life; (b) and (c) a flat surface. FIGURE 34.I
stepped shaft to conical surface;
Surface Treatments, Coatings, and Cleaning
Explosive l-lardening. In explosive hardening, the surfaces are subjected to high transient pressures through the placement and detonation of a layer of an explosive sheet directly on the workpiece surface. The contact pressures that develop as a result can be as high as 35 GPa and can last about 2 to 3 /as. Major increases in surface hardness can be achieved with this method, with very little change (less than 5%) in the shape of the component. Railroad rail surfaces, for example, are explosively hardened.
Mechanical Plating and Cladding
Mechanical Plating. In mechanical plating (also called mechanical coating, impact plating, or peen plating), fine metal particles are compacted over the workpiece surfaces by glass, ceramic, or porcelain beads that are propelled by rotary means (such as tumbling). This process, which is basically one of cold-welding particles onto a surface, typically is used for hardened-steel parts for automobiles, with plating thickness usually less than 25 um. Cladding. In this process, also called clad bonding, metals are bonded with a thin layer of corrosion-resistant metal through the application of pressure by rolls or other means. A typical application is the cladding of aluminum (Alclad), in which a corrosion-resistant layer of aluminum alloy (usually in sheet or tubular form) is clad over an aluminum-alloy body (core). The cladding layer is anodic to the core and usually has a thickness that is less than 10% of the total thickness. Examples of cladding are 2024 aluminum clad with 1230 aluminum, and 3003, 6061, and 7178 aluminum clad with 7072 aluminum. Gther applications are steels clad with stainless-steel or nickel alloys. The cladding material also may be applied with dies (as in cladding steel wire with copper) or explosives. Multiplelayer cladding is also utilized in special applications. Laser cladding consists of the fusion of a different material over the substrate. It has been applied successfully to metals and ceramics, especially for enhanced friction and good wear behavior of the components.
Case Hardening and Hard Facing
Surfaces may be hardened by thermal means in order to improve their frictional and wear properties, as well as their resistance to indentation, erosion, abrasion, and corrosion. The most common methods are described next.
Case Hardening. Traditional methods of case hardening (carhurizing, carhonitriding, cyaniding, nitriding, flame hardening, and induction hardening) are described in Section 4.10 and summarized in Table 4.1. In addition to common heat sources (gas and electricity), an electron beam or laser beam can be used as a heat source in surface hardening of both metals and ceramics. Case hardening, as well as some of the other surface-treatment processes described in this chapter, induces residual stresses on surfaces. The formation of martensite during case hardening causes compressive residual stresses on surfaces. Such stresses are desirable, because they improve the fatigue life of components by delaying the initiation of fatigue cracks. Hard Facing. In this process, a relatively thick layer, edge, or point of wearresistant hard metal is deposited on the workpiece surface by the fusion-welding ~
Section 34. 5
techniques described in Chapter 30. Numerous layers (known as weld overlay) can be deposited to repair worn parts. Hard facing enhances the wear resistance of the materials; hence, such materials are used in the manufacture of tools, dies, and various industrial components. Worn parts also can be hard faced for extended use. Spark Hardening. Hard coatings of tungsten, chromium, or molybdenum carbides can be deposited by an electric arc in a process called spark hardening, electric spar/2 hardening, or electrospar/Q deposition. The deposited layer is typically 250 /.rm thick. Hard-facing alloys can be used as electrodes, rods, wires, or powder in spark hardening. Typical applications for these alloys are as valve seats, oil-well drilling tools, and dies for hot metalworking.
Thermal spraying is a series of processes in which coatings of various metals, alloys, carbides, ceramics, and polymers are applied to metal surfaces by a spray gun with a stream heated by an oxyfuel flame, an electric arc, or a plasma arc. The earliest applications of thermal spraying (in the 1910s) involved metals (hence the term metallizing has also been used), and these processes are under continuous refinement. The surfaces to be sprayed are first cleaned of oil and dirt, and then roughened by, for example, grit blasting, to improve their bond strength (see Section 26.8). The coating material can be in the form of wire, rod, or powder, and when the droplets or particles impact the workpiece, they solidify and bond to the surface. Depending on the process, particle velocities typically range from a low of about 150 to 1000 m/s, but can be higher for special applications. Temperatures are in the range from 3000° to 8000°C. The coating is hard and wear resistant, with a layered structure of deposited material. However, the coating can have a porosity as high as 20% due to entrapped air and oxide particles because of the high temperatures involved. Bond strength depends on the particular process and techniques used and is mostly mechanical in nature (hence the importance of roughening the surface prior to spraying), but can be metallurgical in some cases. Bond strength generally ranges from 7 to 80 MPa, depending on the particular process used. Typical applications of thermal spraying include aircraft engine components (such as those used in rebuilding worn parts), structures, storage tanks, tank cars, rocket motor nozzles, and components that require resistance to wear and corrosion. In an automobile, thermal spraying typically can be applied to crankshafts, valves, fuel-injection nozzles piston rings, and engine blocks. The process is also used in the gas and petrochemical industries, for the repair of worn parts and to restore dimensional accuracy to parts that have not been machined or formed properly. The source of energy in thermal-spraying processes is of two types: combustion and electrical.
Combustion Spraying °
Thermal wire spraying (Fig. 34.Za): The oxyfuel flame melts the wire and deposits it on the surface. The bond is of medium strength, and the process is relatively inexpensive. Thermal metal-powder spraying (Fig. 34_2b): This process is similar to flame wire spraying, but uses a metal powder instead of the wire.
Surface Treatments, Coatings, and Cleaning
Wire or rod
Oxygen Fuel gas
Flame Fuel gas
Molten metal spray
Deposited coating (D)
Spray powder ClfCU|3T'l'lQ
Prepared base material (water cooled)
Plasma Deposited Spray
power to arc
Lsemimolte spray stream
Schematic illustrations of thermal-spray operations: (a) thermal wire spray, (b) thermal metal-powder spray, and lc) plasma spray. FIGURE 34.2
Detonation gun: Controlled and repeated explosions take place by means of an oxyfuel-gas mixture. The detonation gun has a performance similar to that of plasma. High-velocity oxyfuel-gas spraying (HVOF): This process produces a high performance similar to that of the detonation gun, but is less expensive.
Electrical Spraying °
Twin-wire arc: An arc is formed between two consumable Wire electrodes. The resulting bond has good strength, and the process is the least expensive.
Section 34.6 °
Plasma: Either conventional, high-energy, or vacuum (Fig. 34.2c) plasma produces temperatures on the order of 8300°C and results in good bond strength with very low oxide content. Low-pressure plasma spray (LPPS) and vacuum plasma spray both produce coatings with high bond strength and with very low levels of porosity and surface oxides.
Cold Spraying. In this more recent development, the particles to be sprayed are at a lower temperature and are not melted; thus, oxidation is minimal. The spray jet in cold spraying is narrow and highly focused; it has very high impact velocities, thereby improving the bond strength of the particles on the surface.
EXAMPLE 34.1 Repair
of a Worn Turbine-engine Shaft by Thermal Spraying
The shaft of the helical gear for a GE T-38 gas-turbine engine had two worn regions on its nitrided surfaces. The case-hardened depth was 0.3 mm. Even though the helical gears were in good condition, the part was considered scrap because there was no approved method of repair. The worn regions first were machined undersize, grit blasted, and coated with tungsten carbide (12%
cobalt content; see Section 22.5) using the high-velocity oxyfuel-gas thermal-spraying (HVOF) technique. Then the part was finish machined to the dimensions of the original shaft. The total cost of repair was a fraction of the projected cost of replacing the part. Source: Courtesy of Plasma Technology, Inc.
Vapor deposition is a process in which the substrate (workpiece surface) is subjected to chemical reactions by gases that contain chemical compounds of the material to be deposited. The coating thickness is usually a few microns, which is much less than the thicknesses that result from the techniques described in Sections 34.2 and 34.3. The deposited materials can consist of metals, alloys, carbides, nitrides, borides, ceramics, or oxides. Control of the coating composition, thickness, and porosity are important. The substrate may be metal, plastic, glass, or paper. Typical applications for vapor deposition are the coating of cutting tools, drills, reamers, milling cutters, punches, dies, and wear surfaces. There are two major vapor-deposition processes: physical vapor deposition and chemical vapor deposition.
34.6.I Physical Vapor Deposition The three basic types of physical vapor deposition (PVD) processes are (1) vacuum deposition, or arc evaporation; (2) sputtering; and (3) ion plating. These processes are carried out in a high vacuum and at temperatures in the range from 200° to 500°C. In PVD, the particles to be deposited are carried physically to the workpiece, rather than being carried by chemical reactions (as in chemical vapor deposition).
Vacuum Deposition. In vacuum deposition (or evaporation), the metal is evaporated at a high temperature in a vacuum and is deposited on the substrate (which is usually at room temperature or slightly higher for improved bonding). Coatings of uniform thickness can be deposited, even on complex shapes. In arc deposition (PV/ARC), the coating material (cathode) is evaporated by several arc evaporators
Surface Treatments, Coatings, and Cleaning
Plasma Reactive gas
Evaporator Vacuum pump
Power supply Schematic illustration of the physical-vapor(a) deposition process. Note that there are three arc evaporators and the parts to be coated are placed on a tray inside the chamber. FIGURE 34.3
Working gas feed
Target lon flux
v cuum pumps
FIGURE 34 4
.iw i,._i, ,
343) using highly localized electric arcs. The arcs produce a highly reactive plasma, which consists of ionized vapor of the coating material. The vapor condenses on the substrate (anode) and coats it. Applications of this process are both functional (oxidation-resistant coatings for high-temperature applications, electronics, and optics) and decorative (hardware, appliances, and jewelry). Pulsed-laser deposition is a more recent, related process in which the source of energy is a pulsed (Fig.
In sputtering, an electric field ionizes an inert gas (usually argon). The positive ions bombard the coating material (cathode) and cause sputtering Schematic illustration of the sputtering process. (ejection) of its atoms. The atoms then condense on the workpiece, which is heated to improve bonding (Fig. 34.4). In reactive sputtering, the inert gas is replaced by a reactive gas (such as oxygen), in which case the atoms are oxidized and the oxides are deposited. Carbides and nitrides also are deposited by reactive sputtering. Alternatively, very thin polymer coatings can be deposited on metal and polymeric substrates with a reactive gas, causing polymerization of the plasma. Radio-frequency (RF) sputtering is used for nonconductive materials, such as electrical insulators and semiconductor devices.
lon Plating. Ion plating is a generic term that describes various combined processes of sputtering and vacuum evaporation. An electric field causes a glow, generating a plasma (Fig. 34.5). The vaporized atoms in this process are ionized only partially. Ion-beam-enhanced (assisted) deposition is capable of producing thin films as coatings for semiconductor, tribological, and optical applications. Bulky parts can be coated in large chambers using high-current power supplies of 15 kW and voltages of 100,000 DC. Dual ion-beam deposition is a hybrid coating technique that combines PVD with simultaneous ion-beam bombardment. This technique results in good adhesion on metals, ceramics, and polymers. Ceramic bearings and dental instruments are examples of its applications.
Section 34 6
Variable leak Movable shutter
""',,< or higher. Linear and angular measurements are made directly on the screen, which is marked with reference lines and circles. For angular measurements, the screen can be rotated.
35.4.4 Gages This section describes several common gages that have simple solid shapes and cannot be classified as instruments although they are very valuable in metrology. Gage Blocks. Gage blocks are individual square, rectangular, or round blocks of various sizes. For general use, they are made from heat-treated and stress-relieved alloy
Engineering Metrology and Instrumentation
steels. The better gage blocks are made of ceramics (often zirconia) and chromium carbide-unlike steels, these materials do not rust, but they are brittle and must be handled carefully. Angle bloc/as are made the same way and are used for angular gaging. Gage blocks have a flatness within 1.25 /im.
Environmental temperature control is important when gages are used for high-precision measurements.
Projected screen image Clips for
Fixed Gages. These gages are replicas of the shapes of the parts to be measured. Although /Qxed gages are easy to use and inexpensive, they indicate only whether a part is too small or too large compared with an established standard.
Plug gages are commonly used for holes (Figs. 35.1Oa and b). The GO gage is smaller than the NOT GO (or NO GO) gage and slides into any hole that has a dimension smaller than the diameter of the gage. The NOT GO gage must not go into the hole. Two gages are required for such FIGURE 35.9 A bench-model horizontal-beam contour projecmeasurements, although both may be on tor with a 16-in.-diameter (400-mm) screen with 150-W tungsten halogen illumination. Source: Courtesy of L.S. Starrett Company, the same device-either at opposite ends or Precision Optical Division. in two steps at one end (step-type gage). Plug gages also are available, for measuring internal tapers (in which deviations between the gage and the part are indicated by the looseness of the gage), splines, and threads (in which the GO gage must screw into the threaded hole). ° Ring gages (Fig. 35.10c) are used to measure shafts and similar round parts. Ring thread gages are used to measure external threads. The GO and NOT °
_'__ |. || |
Nor GO (C)
35.I0 (a) Plug gage for holes, with GO and NOT GO on opposite ends of the gage. (b) Plug gage with GO and NOT GO on one end. (c) Plain ring gages for gaging round rods. Note the difference in knurled surfaces to identify the two gages. (d) Snap gage with adjustable anvils. FIGURE
Traditional Measuring Methods and Instruments
GO features on these gages are identified by the type of knurling on the outside diameters of the rings. Snap gages (Fig. 35 .10d) commonly are used to measure external dimensions. They are made with adjustable gaging surfaces for use with parts that have different dimensions. One of the gaging surfaces can be set at a different gap from the other, thus making the device a one-unit GO-and-NOT-GO gage.
The basic operation of an air gage (also called a pneumatic gage) is shown in Fig. 35.lla. The gage head (air plug) has two or more holes, typically 1.25 mm in diameter, through which pressurized air (supplied by a constant~pressure line) escapes. The smaller the gap between the gage and the hole, the more difficult it is for the air to escape, and hence, the higher is the back pressure. The back pressure, which is sensed Air Gages.
i) i' i ’
Pressure gage Part
Air filter (H)
Pneumatic lines Workpiece (crankshaft)
(a) Schematic illustration of the principle of an air gage. (b) Illustration of an air-gage system used to measure the main bearing dimension on a crankshaft. (c) A conical head for air gaging; note the three small airholes on the conical surface. Source: (b) Courtesy of Mahr Federal, Inc. (c) Courtesy of Stotz Gaging Co.
Engineering Metrology and Instrumentation
and indicated by a pressure gage,
calibrated to measure the dimensional variations
The air gage can be rotated during use to indicate and measure any out-ofroundess of the hole. The outside diameters of parts (such as pins and shafts) also can be measured when the air plug is in the shape of a ring slipped over the part. In cases where a ring is not suitable, a fork-shaped gage head (with the airholes at the tips) can be used (Fig. 35.11b). Various shapes of air heads, such as the conical head shown in Fig. 35.11c, can be prepared for use in specialized applications on parts with different geometric features. Air gages are easy to use, and the resolution can be as fine as 0.125 um. If the surface roughness of the part is too high, the readings may be unreliable. The compressed-air supply must be clean and dry for proper operation. The part being measured does not have to be free of dust, metal particles, or similar contaminants, because the air will blow them away. The noncontacting nature and the low pressure of an air gage has the benefit of not distorting or damaging the measured part, as could be the case with mechanical gages-thus giving erroneous readings.
Modern Measuring Instruments and Machines
wide variety of measuring instruments and gages has been developed. They range from simple, hand-operated devices to computer-controlled machines with very large workspaces. A
Electronic Gages. Unlike mechanical systems, electronic gages sense the movement of the contacting pointer through changes in the electrical resistance of a strain gage, inductance, or capacitance. The electrical signals are then converted and displayed as linear dimensions with a digital readout. A handheld electronic gage for measuring bore diameters is shown in Fig. 35.12. When its handle is squeezed slightly, the tool can be inserted into the bore, and the bore diameter is read directly. A microprocessorassisted electronic gage for measuring vertical length is shown in Fig. 35.13. A commonly used electronic gage is the linear-variable differential transformer (LVDT), for measuring small displacements. Electronic caliper gages with diamondcoated edges are available. The chemical vapor deposition (CVD) coating on these gages has a wear resistance superior to that of steel or tungsten-carbide edges; it also resists corrosion. Although they are more expensive than other types of gages, electronic gages have advantages in ease of operation, rapid response, a digital readout, less possibility of human error, versatility, flexibility, and the capability to be integrated into automated systems through microprocessors and computers.
35.l2 An electronic gage for measuring bore diameters. The measuring head is equipped with three carbide-tipped steel pins for wear resistance. The LED display reads 29.158 mm. Source: Courtesy of TESA SA. FIGURE
Laser Micrometers. In this instrument, a laser beam scans the workpiece (Fig. 35.14), typically at a rate of 350 times per second. Laser micrometers are capable of resolutions as high as 0.125 um. They are suitable not only for stationary parts, but also for in-line measurement of stationary, rotating, or vibrating parts, as well as parts in continuous, highspeed production. In addition, because there is no physical contact, they can measure parts that are at elevated temperatures or are too flexible to be measured by other means. The laser beams can be of various types (such as scanning or
Modern Measuring Instruments and Machines
rastoring for stationary parts), yielding point-cloud descriptions of part surfaces. Laser micrometers are of the shadow type or are charge-coupled device (CCD) based for in-line measurement while a part is in production. Laser micrometers are available with various capacities and features. They can be handheld for manual operation, or they can be mounted on and integrated with computer-controlled machines and statistical-process control units. Laser lnterferometry. This technique is used to check and calibrate machine tools for various geometric features during assembly. The method has better accuracies than those of gages or indicators. Laser interferometers are also used to automatically compensate for positioning errors in coordinatemeasuring machines and computer-numerical control machines.
Photoelectric Digital Length Measurement. This type of measurement is done by an instrument that can measure the overall dimensions, thickness, and depth of a variety of parts. Resolution settings can range from
35.5.l Coordinate-measuring Machines
FIGURE 35.l3 An electronic verticallength measuring instrument with a resolution of 1 /.tm(40 pin). Source: Courtesy of TESA SA.
As schematically shown in Fig. 35 .15 a, a coordinate-measuring machine (CMM) consists basically of a platform on which the workpiece being measured is placed and is then moved linearly or rotated. A probe (Fig. 35 .15 b; see also Fig. 25.6) is attached to a head (capable of various movements) and records all
measurements. In addition to the tactile probe shown, other types of probes are scanning, laser (Fig. 35.15c), and vision probes, all of which are nontactile. A CMM for inspection of a typical part is shown in Fig. 35.15d. Coordinate-measuring machines are very versatile and capable of recording measurements of complex profiles with high resolution (0.25 um) and high speed. They are built rigidly and ruggedly to resist environmental effects in manufacturing plants, such as temperature variations and vibration. They can be placed close to machine tools for efficient inspection and rapid feedback; that way, processing parameters are corrected before the next part is made. Although large CMMS can be expensive, most machines with a touch probe and computer-controlled three-dimensional movement are suitable for use in small shops and generally cost under $20,000.
x Laser beam
Direct measurement of
diameter D (H)
35.l4 (a) and (b) Two types of measurements made with a laser scan micrometer. Two types of laser micrometers. Note that the instrument in the front scans the part (placed in the opening) in one dimension; the larger instrument scans the part in two dimensions. Source: Courtesy of BETA LaserMike. FIGURE (c)
I0 0 I
Engineering Metrology and Instrumentation
z-axis fine-feed knob x-axis fine-feed knob
Probe adapter Clamp knobs for x, y, and zaxes
pera Iona pane y-axis fine-feed knob
(a) Schematic illustration of a coordinate-measuring machine. (b) A touch signal probe. (c) Examples of laser probes. (d) A coordinate-measuring machine with a complex part being measured. Source: (b) through (d) Courtesy of Mitutoyo America Corp.
Coordinate-measuring Machine for Car Bodies
large horizontal CNC coordinate-measuring machine used to measure all dimensions ofa car body is shown in Fig. 35.16. This machine has a measuring range of 6 X 1.6 X 2.4 m high and a resolution of 0.1 /rm. The system has temperature compensation within a range from 16° to 26°C to maintain A
measurement accuracy. For efficient measurements, the machine has two heads with touch-trigger probes that are controlled simultaneously and have full threedimensional movements. The measuring speed is 5 mm/s. The probes are software controlled, and the machine is equipped with safety devices to prevent the
Automated Measurement and Inspection
A large coordinate-measuring machine with two heads measuring various dimensions on a car body.
probes from inadvertently hitting any part of the car body during their movements. The equipment shown around the base of the machine includes supporting
hardware and software that controls all movements and records all measurements Source: Courtesy of Mitutoyo America Corporation
Automated Measurement and Inspection
Automated measurement and inspection is based on various online sensor systems that monitor the dimensions of parts while they are being made and, if necessary, use these measurements as input to make corrections (Section 37.7). Manufacturing cells and flexible manufacturing systems (Chapter 39) have led to the adoption of advanced measuring techniques and systems. To appreciate the importance of online monitoring of dimensions, consider the following question: If a machine has been producing a certain part with acceptable dimensions, what factors contribute to the subsequent deviation in the dimensions of the same part produced by the same machine? There are several technical, as Well as human, factors involved: °
Static and dynamic deflections of the machine because of vibrations and fluctuating forces are caused by machine characteristics and variations in the properties and dimensions of the incoming material. Distortion of the machine because of thermal effects are caused by such factors as changes in the temperature of the environment, changes of metalworking fluids, and changes of machine bearings and various components. Wear of tools, dies, and molds can affect the dimensional accuracy of the parts produced. Human errors and miscalculations cause problems.
As a result of these factors, the dimensions of parts tinuous monitoring during production necessary.
thus making con-
I0 2 I
Engineering Metrology and Instrumentation
General Characteristics and Selection of Measuring Instruments
The characteristics and quality of measuring instruments are generally described by various specific terms, defined as follows (in alphabetical order): ° ° ° ° ° ° ° ° ° °
° ° °
Accuracy: The degree of agreement of the measured dimension with its true magnitude. Amplification: The ratio of instrument output to the input dimension; also called rnagnihcation. Calibration: The adjustment or setting of an instrument to give readings that are accurate within a reference standard. Drift: An instrument’s capability to maintain its calibration over time; also called stability. Linearity: The accuracy of the readings of an instrument over its full working range. Magnification: The ratio of instrument output to the input dimension; also called amplification. Precision: Degree to which an instrument gives repeated measurement of the same standard. Repeat accuracy: The same as accuracy, but repeated many times. Resolution: Smallest dimension that can be read on an instrument. Rule of 10 (gage rna/eer’s rule): An instrument or gage should be 10 times more accurate than the dimensional tolerances of the part being measured. A factor of 4 is known as the rnil standard rule. Sensitivity: Smallest difference in dimension that an instrument can distinguish or detect. Speed of response: How rapidly an instrument indicates a measurement, particularly when a number of parts are measured in rapid succession. Stability: An instrument’s capability to maintain its calibration over time; also called drift.
The selection of an appropriate measuring instrument for a particular application also depends on (a) the size and type of parts to be measured, (b) the environment (temperature, humidity, dust, and so on), (c) the operator skills required, and (d) the cost of equipment.
Geometric Dimensioning and Tolerancing
Individually manufactured parts and components eventually are assembled into products. We take it for granted that when a thousand lawn mowers are manufactured and assembled, each part of the mower will mate properly with its intended components. For example, the wheels of the lawn mower will slip easily into their axles, or the pistons will fit properly into the cylinders, being neither too tight nor too loose. Likewise, when we have to replace a broken or worn bolt on an old machine, we purchase an identical bolt. We are confident from similar experiences in the past that the new bolt will fit properly in the machine. The reason we feel confident is that the bolt is manufactured according to certain standards and the dimensions of all similar bolts will vary by only a small, specified amount that do not affect their function. In other words, all bolts are manufactured within a certain range of dimensional tolerance; thus, all similar bolts are interchangeable. We also expect that the new bolt will function satisfactorily for a certain length of time, unless it is abused
Geometric Dimensionmg and Tolerancmg
or misused. Bolts are periodically subjected to various tests during their production
to make sure that their quality is within certain specifications.
Dimensional Tolerance. Dimensional tolerance is defined as the permissible or acceptable variation in the dimensions (height, width, depth, diameter, and angles) of a part. The root of the word “tolerance” is the Latin tolerare, meaning “to endure” or “to put up with.” Tolerances are unavoidable, because it is virtually impossible and unnecessary to manufacture two parts that have precisely the same dimensions. Furthermore, because close dimensional tolerances can increase the product cost significantly, a narrow tolerance range is economically undesirable. However, for some parts, close tolerances are necessary for their proper functioning and are worth the added expense associated with narrow tolerance ranges. Examples are precision measuring instruments and gages, hydraulic pistons, and bearings for aircraft engines.
Measuring dimensional tolerances and features of parts rapidly and reliably can parts on a Boeing 747-400 aircraft requires the measurement of about 25 features, representing a total of 150 million measurements. Surveys have shown that the dimensional tolerances on state-of-the-art manufactured parts are shrinking by a factor of 3 every 10 years and that this trend will continue. It is estimated that accuracies of (a) conventional turning and milling machines will rise from the present 7.5 to 1 /im, (b) diamond-wheel wafer-slicing machines for semiconductor fabrication to 0.25 /sum, (c) precision diamond turning machines to 0.01 um, and (d) ultraprecision ion-beam machines to less than 0.001 /J.m. (See also Fig. 25.16.) be a challenging task. For example, each of the 6 million
U # (D
E '_ U
HE at BED P-10 """"'O O°'°E"'3° QQ..
5 _Q V9